Presentation on theme: "WELDING PROCESSES Arc Welding Resistance Welding Oxyfuel Gas Welding"— Presentation transcript:
1 WELDING PROCESSES Arc Welding Resistance Welding Oxyfuel Gas Welding Other Fusion Welding ProcessesSolid State WeldingWeld QualityWeldability
2 Two Categories of Welding Processes Fusion welding - coalescence is accomplished by melting the two parts to be joined, in some cases adding filler metal to the jointExamples: arc welding, resistance spot welding, oxyfuel gas weldingSolid state welding - heat and/or pressure are used to achieve coalescence, but no melting of base metals occurs and no filler metal is addedExamples: forge welding, diffusion welding, friction welding
3 Arc Welding (AW)A fusion welding process in which coalescence of the metals is achieved by the heat from an electric arc between an electrode and the workElectric energy from the arc produces temperatures ~ 10,000 F (5500 C), hot enough to melt any metalMost AW processes add filler metal to increase volume and strength of weld joint
4 What is an Electric Arc?An electric arc is a discharge of electric current across a gap in a circuitIt is sustained by an ionized column of gas (plasma) through which the current flowsTo initiate the arc in AW, electrode is brought into contact with work and then quickly separated from it by a short distance
5 Figure 31.1 Basic configuration of an arc welding process. A pool of molten metal is formed near electrode tip, and as electrode is moved along joint, molten weld pool solidifies in its wakeFigure Basic configuration of an arc welding process.
6 Two Basic Types of AW Electrodes Consumable – consumed during welding processSource of filler metal in arc weldingNonconsumable – not consumed during welding processFiller metal must be added separately
7 Consumable Electrodes Forms of consumable electrodesWelding rods (a.k.a. sticks) are 9 to 18 inches and 3/8 inch or less in diameter and must be changed frequentlyWeld wire can be continuously fed from spools with long lengths of wire, avoiding frequent interruptionsIn both rod and wire forms, electrode is consumed by arc and added to weld joint as filler metal
8 Nonconsumable Electrodes Made of tungsten which resists meltingGradually depleted during welding (vaporization is principal mechanism)Any filler metal must be supplied by a separate wire fed into weld pool
9 Arc ShieldingAt high temperatures in AW, metals are chemically reactive to oxygen, nitrogen, and hydrogen in airMechanical properties of joint can be seriously degraded by these reactionsTo protect operation, arc must be shielded from surrounding air in AW processesArc shielding is accomplished by:Shielding gases, e.g., argon, helium, CO2Flux
10 FluxA substance that prevents formation of oxides and other contaminants in welding, or dissolves them and facilitates removalProvides protective atmosphere for weldingStabilizes arcReduces spattering
11 Various Flux Application Methods Pouring granular flux onto welding operationStick electrode coated with flux material that melts during welding to cover operationTubular electrodes in which flux is contained in the core and released as electrode is consumed
12 Power Source in Arc Welding Direct current (DC) vs. Alternating current (AC)AC machines less expensive to purchase and operate, but generally restricted to ferrous metalsDC equipment can be used on all metals and is generally noted for better arc control
13 Consumable Electrode AW Processes Shielded Metal Arc WeldingGas Metal Arc WeldingFlux‑Cored Arc WeldingElectrogas WeldingSubmerged Arc Welding
14 Shielded Metal Arc Welding (SMAW) Uses a consumable electrode consisting of a filler metal rod coated with chemicals that provide flux and shieldingSometimes called "stick welding"Power supply, connecting cables, and electrode holder available for a few thousand dollars
15 Shielded Metal Arc Welding Figure Shielded metal arc welding (SMAW).
16 Shielded Metal Arc Welding Figure 31.2 Shielded metal arc welding (stick welding) performed by a (human) welder (photo courtesy of Hobart Brothers Co.).
17 SMAW ApplicationsUsed for steels, stainless steels, cast irons, and certain nonferrous alloysNot used or rarely used for aluminum and its alloys, copper alloys, and titanium
18 Gas Metal Arc Welding (GMAW) Uses a consumable bare metal wire as electrode and shielding accomplished by flooding arc with a gasWire is fed continuously and automatically from a spool through the welding gunShielding gases include inert gases such as argon and helium for aluminum welding, and active gases such as CO2 for steel weldingBare electrode wire plus shielding gases eliminate slag on weld bead - no need for manual grinding and cleaning of slag
20 GMAW Advantages over SMAW Better arc time because of continuous wire electrodeSticks must be periodically changed in SMAWBetter use of electrode filler metal than SMAWEnd of stick cannot be used in SMAWHigher deposition ratesEliminates problem of slag removalCan be readily automated
21 Flux‑Cored Arc Welding (FCAW) Adaptation of shielded metal arc welding, to overcome limitations of stick electrodesElectrode is a continuous consumable tubing (in coils) containing flux and other ingredients (e.g., alloying elements) in its coreTwo versions:Self‑shielded FCAW - core includes compounds that produce shielding gasesGas‑shielded FCAW - uses externally applied shielding gases
22 Flux-Cored Arc Welding Figure Flux‑cored arc welding. Presence or absence of externally supplied shielding gas distinguishes the two types: (1) self‑shielded, in which core provides ingredients for shielding, and (2) gas‑shielded, which uses external shielding gases.
23 Electrogas Welding (EGW) Uses a continuous consumable electrode, either flux‑cored wire or bare wire with externally supplied shielding gases, and molding shoes to contain molten metalWhen flux‑cored electrode wire is used and no external gases are supplied, then special case of self‑shielded FCAWWhen a bare electrode wire used with shielding gases from external source, then special case of GMAW
24 Electrogas WeldingFigure Electrogas welding using flux‑cored electrode wire: (a) front view with molding shoe removed for clarity, and (b) side view showing molding shoes on both sides.
25 Submerged Arc Welding (SAW) Uses a continuous, consumable bare wire electrode, with arc shielding provided by a cover of granular fluxElectrode wire is fed automatically from a coilFlux introduced into joint slightly ahead of arc by gravity from a hopperCompletely submerges operation, preventing sparks, spatter, and radiation
27 SAW Applications and Products Steel fabrication of structural shapes (e.g., I‑beams)Seams for large diameter pipes, tanks, and pressure vesselsWelded components for heavy machineryMost steels (except hi C steel)Not good for nonferrous metals
29 Gas Tungsten Arc Welding (GTAW) Uses a non-consumable tungsten electrode and an inert gas for arc shieldingMelting point of tungsten = 3410C (6170F)A.k.a. Tungsten Inert Gas (TIG) weldingIn Europe, called "WIG welding"Used with or without a filler metalWhen filler metal used, it is added to weld pool from separate rod or wireApplications: aluminum and stainless steel most common
30 Gas Tungsten Arc Welding Figure Gas tungsten arc welding.
31 Advantages / Disadvantages of GTAW High quality welds for suitable applicationsNo spatter because no filler metal through arcLittle or no post-weld cleaning because no fluxDisadvantages:Generally slower and more costly than consumable electrode AW processes
32 Plasma Arc Welding (PAW) Special form of GTAW in which a constricted plasma arc is directed at weld areaTungsten electrode is contained in a nozzle that focuses a high velocity stream of inert gas (argon) into arc region to form a high velocity, intensely hot plasma arc streamTemperatures in PAW reach 28,000C (50,000F), due to constriction of arc, producing a plasma jet of small diameter and very high energy density
34 Advantages / Disadvantages of PAW Good arc stabilityBetter penetration control than other AWHigh travel speedsExcellent weld qualityCan be used to weld almost any metalsDisadvantages:High equipment costLarger torch size than other AWTends to restrict access in some joints
35 Resistance Welding (RW) A group of fusion welding processes that use a combination of heat and pressure to accomplish coalescenceHeat generated by electrical resistance to current flow at junction to be weldedPrincipal RW process is resistance spot welding (RSW)
36 Resistance WeldingFigure Resistance welding, showing the components in spot welding, the main process in the RW group.
37 Components in Resistance Spot Welding Parts to be welded (usually sheet metal)Two opposing electrodesMeans of applying pressure to squeeze parts between electrodesPower supply from which a controlled current can be applied for a specified time duration
38 Advantages / Drawbacks of RW No filler metal requiredHigh production rates possibleLends itself to mechanization and automationLower operator skill level than for arc weldingGood repeatability and reliabilityDisadvantages:High initial equipment costLimited to lap joints for most RW processes
39 Resistance Spot Welding (RSW) Resistance welding process in which fusion of faying surfaces of a lap joint is achieved at one location by opposing electrodesUsed to join sheet metal parts using a series of spot weldsWidely used in mass production of automobiles, appliances, metal furniture, and other products made of sheet metalTypical car body has ~ 10,000 spot weldsAnnual production of automobiles in the world is measured in tens of millions of units
40 Spot Welding CycleFigure (a) Spot welding cycle, (b) plot of squeezing force & current in cycle (1) parts inserted between electrodes, (2) electrodes close, force applied, (3) current on, (4) current off, (5) electrodes opened.
41 Resistance Seam Welding (RSEW) Uses rotating wheel electrodes to produce a series of overlapping spot welds along lap jointCan produce air‑tight jointsApplications:Gasoline tanksAutomobile mufflersVarious other sheet metal containers
43 Resistance Projection Welding (RPW) A resistance welding process in which coalescence occurs at one or more small contact points on partsContact points determined by design of parts to be joinedMay consist of projections, embossments, or localized intersections of parts
44 Resistance Projection Welding Figure Resistance projection welding (RPW): (1) start of operation, contact between parts is at projections; (2) when current is applied, weld nuggets similar to spot welding are formed at the projections.
45 Oxyfuel Gas Welding (OFW) Group of fusion welding operations that burn various fuels mixed with oxygenOFW employs several types of gases, which is the primary distinction among the members of this groupOxyfuel gas is also used in flame cutting torches to cut and separate metal plates and other partsMost important OFW process is oxyacetylene welding
46 Oxyacetylene Welding (OAW) Fusion welding performed by a high temperature flame from combustion of acetylene and oxygenFlame is directed by a welding torchFiller metal is sometimes addedComposition must be similar to base metalFiller rod often coated with flux to clean surfaces and prevent oxidation
47 Figure 31.21 A typical oxyacetylene welding operation (OAW).
48 Acetylene (C2H2)Most popular fuel among OFW group because it is capable of higher temperatures than any other ‑ up to 3480C (6300F)Two stage chemical reaction of acetylene and oxygen:First stage reaction (inner cone of flame):C2H2 + O2 2CO + H2 + heatSecond stage reaction (outer envelope):2CO + H O2 2CO2 + H2O + heat
49 Oxyacetylene TorchMaximum temperature reached at tip of inner cone, while outer envelope spreads out and shields work surfaces from atmosphereFigure The neutral flame from an oxyacetylene torch indicating temperatures achieved.
50 Alternative Gases for OFW Methylacetylene‑Propadiene (MAPP)HydrogenPropylenePropaneNatural Gas
51 Other Fusion Welding Processes FW processes that cannot be classified as arc, resistance, or oxyfuel weldingUse unique technologies to develop heat for meltingApplications are typically uniqueProcesses include:Electron beam weldingLaser beam weldingElectroslag weldingThermit welding
52 Electron Beam Welding (EBW) Fusion welding process in which heat for welding is provided by a highly‑focused, high‑intensity stream of electrons striking work surfaceElectron beam gun operates at:High voltage (e.g., 10 to 150 kV typical) to accelerate electronsBeam currents are low (measured in milliamps)Power in EBW not exceptional, but power density is
54 Laser Beam Welding (LBW) Fusion welding process in which coalescence is achieved by energy of a highly concentrated, coherent light beam focused on jointLaser = "light amplification by stimulated emission of radiation"LBW normally performed with shielding gases to prevent oxidationFiller metal not usually addedHigh power density in small area, so LBW often used for small parts
55 Comparison: LBW vs. EBW No vacuum chamber required for LBW No x‑rays emitted in LBWLaser beams can be focused and directed by optical lenses and mirrorsLBW not capable of the deep welds and high depth‑to‑width ratios of EBWMaximum LBW depth = ~ 19 mm (3/4 in), whereas EBW depths = 50 mm (2 in)
56 Thermit Welding (TW)FW process in which heat for coalescence is produced by superheated molten metal from the chemical reaction of thermiteThermite = mixture of Al and Fe3O4 fine powders that produce an exothermic reaction when ignitedAlso used for incendiary bombsFiller metal obtained from liquid metalProcess used for joining, but has more in common with casting than welding
57 Thermit WeldingFigure Thermit welding: (1) Thermit ignited; (2) crucible tapped, superheated metal flows into mold; (3) metal solidifies to produce weld joint.
58 TW Applications Joining of railroad rails Repair of cracks in large steel castings and forgingsWeld surface is often smooth enough that no finishing is required
59 Solid State Welding (SSW) Coalescence of part surfaces is achieved by:Pressure alone, orHeat and pressureIf both heat and pressure are used, heat is not enough to melt work surfacesFor some SSW processes, time is also a factorNo filler metal is addedEach SSW process has its own way of creating a bond at the faying surfaces
60 Success Factors in SSWEssential factors for a successful solid state weld are that the two faying surfaces must be:Very cleanIn very close physical contact with each other to permit atomic bonding
61 SSW Advantages over FW Processes If no melting, then no heat affected zone, so metal around joint retains original propertiesMany SSW processes produce welded joints that bond the entire contact interface between two parts rather than at distinct spots or seamsSome SSW processes can be used to bond dissimilar metals, without concerns about relative melting points, thermal expansions, and other problems that arise in FW
63 Forge WeldingWelding process in which components to be joined are heated to hot working temperature range and then forged together by hammering or similar meansHistoric significance in development of manufacturing technologyProcess dates from about 1000 B.C., when blacksmiths learned to weld two pieces of metalOf minor commercial importance today except for its variants
64 Roll Welding (ROW)SSW process in which pressure sufficient to cause coalescence is applied by means of rolls, either with or without external heatVariation of either forge welding or cold welding, depending on whether heating of workparts is done prior to processIf no external heat, called cold roll weldingIf heat is supplied, hot roll welding
66 Roll Welding Applications Cladding stainless steel to mild or low alloy steel for corrosion resistanceBimetallic strips for measuring temperature"Sandwich" coins for U.S mint
67 Diffusion Welding (DFW) SSW process uses heat and pressure, usually in a controlled atmosphere, with sufficient time for diffusion and coalescence to occurTemperatures 0.5 TmPlastic deformation at surfaces is minimalPrimary coalescence mechanism is solid state diffusionLimitation: time required for diffusion can range from seconds to hours
68 DFW ApplicationsJoining of high‑strength and refractory metals in aerospace and nuclear industriesCan be used to join either similar and dissimilar metalsFor joining dissimilar metals, a filler layer of different metal is often sandwiched between base metals to promote diffusion
69 Explosion Welding (EXW) SSW process in which rapid coalescence of two metallic surfaces is caused by the energy of a detonated explosiveNo filler metal usedNo external heat appliedNo diffusion occurs - time is too shortBonding is metallurgical, combined with mechanical interlocking that results from a rippled or wavy interface between the metals
70 Explosive WeldingCommonly used to bond two dissimilar metals, in particular to clad one metal on top of a base metal over large areasFigure Explosive welding (EXW): (1) setup in the parallel configuration, and (2) during detonation of the explosive charge.
71 Friction Welding (FRW) SSW process in which coalescence is achieved by frictional heat combined with pressureWhen properly carried out, no melting occurs at faying surfacesNo filler metal, flux, or shielding gases normally usedProcess yields a narrow HAZCan be used to join dissimilar metalsWidely used commercial process, amenable to automation and mass production
72 Friction WeldingFigure Friction welding (FRW): (1) rotating part, no contact; (2) parts brought into contact to generate friction heat; (3) rotation stopped and axial pressure applied; and (4) weld created.
73 Applications / Limitations of FRW Shafts and tubular partsIndustries: automotive, aircraft, farm equipment, petroleum and natural gasLimitations:At least one of the parts must be rotationalFlash must usually be removedUpsetting reduces the part lengths (which must be taken into consideration in product design)
74 Ultrasonic Welding (USW) Two components are held together, oscillatory shear stresses of ultrasonic frequency are applied to interface to cause coalescenceOscillatory motion breaks down any surface films to allow intimate contact and strong metallurgical bonding between surfacesAlthough heating of surfaces occurs, temperatures are well below TmNo filler metals, fluxes, or shielding gasesGenerally limited to lap joints on soft materials such as aluminum and copper
75 Ultrasonic WeldingFigure Ultrasonic welding (USW): (a) general setup for a lap joint; and (b) close‑up of weld area.
76 USW ApplicationsWire terminations and splicing in electrical and electronics industryEliminates need for solderingAssembly of aluminum sheet metal panelsWelding of tubes to sheets in solar panelsAssembly of small parts in automotive industry
77 WeldabilityCapacity of a metal or combination of metals to be welded into a suitably designed structure, and for the resulting weld joint(s) to possess the required metallurgical properties to perform satisfactorily in intended serviceGood weldability characterized by:Ease with which welding process is accomplishedAbsence of weld defectsAcceptable strength, ductility, and toughness in welded joint
Your consent to our cookies if you continue to use this website.